# CHAPTER 4: IMPERFECTIONS IN SOLIDS

```CHAPTER 5:
IMPERFECTIONS IN SOLIDS
• What types of defects arise in solids?
• Can the number and type of defects be varied
and controlled?
• How do defects affect material properties?
• Are defects undesirable?
• How do point defects in ceramics differ from those
in metals?
• In ceramics, how are impurities accommodated
in the lattice and how do they affect properties?
1
TYPES OF IMPERFECTIONS
• Vacancy atoms
• Interstitial atoms
• Substitutional atoms
Point defects
• Dislocations
Line defects
• Grain Boundaries
Area defects
2
POINT DEFECTS
• Vacancies:
-vacant atomic sites in a structure.
distortion
of planes
Vacancy
• Self-Interstitials:
-&quot;extra&quot; atoms positioned between atomic sites.
distortion
of planes
selfinterstitial
3
EQUIL. CONCENTRATION:
POINT DEFECTS
• Equilibrium concentration varies with temperature!
No. of defects
Activation energy
Q 
ND 
exp 
 D 

 kT 
N
No. of potential
Temperature
defect sites.
Boltzmann's constant
(1.38 x 10 -23 J/atom K)
(8.62 x 10 -5 eV/atom K)
Each lattice site
is a potential
vacancy site
4
MEASURING ACTIVATION
ENERGY
• We can get Q from
an experiment.
• Measure this...
• Replot it...
ND
ln
N
1
slope
-QD/k
1/T
5
ESTIMATING VACANCY CONC.
• Find the equil. # of vacancies in 1m 3 of Cu at 1000C.
• Given:
0.9eV/atom
Q 
ND
 exp 
 D 
= 2.7 &middot; 10-4
 kT 
N
For 1m 3, N =
1273K
8.62 x 10-5 eV/atom-K
NA
x 1m3 = 8.0 x 1028 sites
 x
ACu
6
OBSERVING EQUIL. VACANCY CONC.
• Low energy electron
microscope view of
a (110) surface of NiAl.
• Increasing T causes
surface island of
atoms to grow.
• Why? The equil. vacancy
conc. increases via atom
motion from the crystal
to the surface, where
they join the island.
Click on image to animate
Reprinted with permission from Nature (K.F.
McCarty, J.A. Nobel, and N.C. Bartelt, &quot;Vacancies in
Solids and the Stability of Surface Morphology&quot;,
Nature, Vol. 412, pp. 622-625 (2001). Image is
5.75 mm by 5.75 mm.) Copyright (2001) Macmillan
Publishers, Ltd.
7
DEFECTS IN CERAMIC
STRUCTURES
• Frenkel Defect
--a cation is out of place.
• Shottky Defect
--a paired set of cation and anion vacancies.
Callister 5e. (Fig. 13.20 is from
W.G. Moffatt, G.W. Pearsall,
and J. Wulff, The Structure and
Properties of Materials, Vol. 1,
Structure, John Wiley and
Sons, Inc., p. 78.) See Fig.
12.21, Callister 6e.
• Equilibrium concentration of defects ~ e
QD / kT
8
POINT DEFECTS IN ALLOYS
Two outcomes if impurity (B) added to host (A):
• Solid solution of B in A (i.e., random dist. of point defects)
OR
Substitutional alloy
(e.g., Cu in Ni)
Interstitial alloy
(e.g., C in Fe)
• Solid solution of B in A plus particles of a new
phase (usually for a larger amount of B)
Second phase particle
--different composition
--often different structure.
9
ALLOYING A SURFACE
• Low energy electron
microscope view of
a (111) surface of Cu.
• Sn islands move along
the surface and &quot;alloy&quot;
the Cu with Sn atoms,
to make &quot;bronze&quot;.
• The islands continually
move into &quot;unalloyed&quot;
regions and leave tiny
bronze particles in
their wake.
• Eventually, the islands
disappear.
Click on image to animate
Reprinted with permission from: A.K. Schmid,
N.C. Bartelt, and R.Q. Hwang, &quot;Alloying at
Surfaces by the Migration of Reactive TwoDimensional Islands&quot;, Science, Vol. 290, No.
5496, pp. 1561-64 (2000). Field of view is 1.5
mm and the temperature is 290K.
10
IMPURITIES
• Impurities must also satisfy charge balance
• Ex: NaCl
• Substitutional cation impurity
• Substitutional anion impurity
O2-
initial geometry
ClClO2- impurity
anion vacancy
resulting geometry
11
COMPOSITION
Definition: Amount of impurity (B) and host (A)
in the system.
Two descriptions:
• Weight %
• Atom %
• Conversion between wt % and at% in an A-B alloy:
CB =
C'BAB
C'AAA + C'BAB
x 100
• Basis for conversion:
12
LINE DEFECTS
Dislocations:
• are line defects,
• cause slip between crystal plane when they move,
• produce permanent (plastic) deformation.
Schematic of a Zinc (HCP):
• before deformation
• after tensile elongation
slip steps
13
INCREMENTAL SLIP
• Dislocations slip planes incrementally...
• The dislocation line (the moving red dot)...
...separates slipped material on the left
from unslipped material on the right.
Simulation of dislocation
motion from left to right
as a crystal is sheared.
Click on image to animate
(Courtesy P.M. Anderson)
14
BOND BREAKING AND
REMAKING
• Dislocation motion requires the successive bumping
of a half plane of atoms (from left to right here).
• Bonds across the slipping planes are broken and
Atomic view of edge
dislocation motion from
left to right as a crystal
is sheared.
(Courtesy P.M. Anderson)
Click on image to animate
15
AREA DEFECTS: GRAIN
BOUNDARIES
Grain boundaries:
•
•
•
•
are boundaries between crystals.
are produced by the solidification process, for example.
have a change in crystal orientation across them.
impede dislocation motion.
Metal Ingot
Schematic
~ 8cm
grain
boundaries
Adapted from Fig. 4.7, Callister 6e.
heat
flow
Adapted from Fig. 4.10, Callister 6e. (Fig.
4.10 is from Metals Handbook, Vol. 9, 9th edition,
Metallography and Microstructures, Am. Society for
Metals, Metals Park, OH, 1985.)
16
OPTICAL MICROSCOPY (1)
• Useful up to 2000X magnification.
• Polishing removes surface features (e.g., scratches)
• Etching changes reflectance, depending on crystal
orientation.
close-packed planes
Adapted from Fig. 4.11(b) and (c),
Callister 6e. (Fig. 4.11(c) is courtesy
of J.E. Burke, General Electric Co.
micrograph of
Brass (Cu and Zn)
0.75mm
17
OPTICAL MICROSCOPY (2)
Grain boundaries...
• are imperfections,
• are more susceptible
to etching,
• may be revealed as
dark lines,
• change direction in a
polycrystal.
and (b), Callister 6e.
(Fig. 4.12(b) is courtesy
of L.C. Smith and C.
Bureau of Standards,
Washington, DC [now the
National Institute of
Standards and
Technology, Gaithersburg,
MD].)
18
SCANNING TUNNELING
MICROSCOPY
• Atoms can be arranged and imaged!
Photos produced from
the work of C.P. Lutz,
Zeppenfeld, and D.M.
Eigler. Reprinted with
permission from
Machines Corporation,
Carbon monoxide
molecules arranged
on a platinum (111)
surface.
Iron atoms
arranged on a
copper (111)
surface. These
Kanji characters
represent the word
“atom”.
19
SUMMARY
• Point, Line, and Area defects arise in solids.
• The number and type of defects can be varied
and controlled (e.g., T controls vacancy conc.)
• Defects affect material properties (e.g., grain
boundaries control crystal slip).
• Defects may be desirable or undesirable
(e.g., dislocations may be good or bad, depending
on whether plastic deformation is desirable or not.)
20
ANNOUNCEMENTS